1 Chemical Substances and Biological Agents Studies and Research Projects REPORT R-656 Engineered Nanoparticles Current Knowledge about OHS Risks and Second Edition Claude Ostiguy Brigitte Roberge Catherine Woods Brigitte Soucy
2 Established in Québec since 1980, the Institut de recherche Robert-Sauvé en santé et en sécurité du travail (IRSST) is a scientific research organization known for the quality of its work and the expertise of its personnel. OUR RESEARCH is working for you! Mission To contribute, through research, to the prevention of industrial accidents and occupational diseases as well as to the rehabilitation of affected workers. To offer the laboratory services and expertise necessary for the activities of the public occupational health and safety prevention network. To disseminate knowledge, and to act as scientific benchmark and expert. Funded by the Commission de la santé et de la sécurité du travail, the IRSST has a board of directors made up of an equal number of employer and worker representatives. To find out more Visit our Web site for complete up-to-date information about the IRSST. All our publications can be downloaded at no charge. To obtain the latest information on the research carried out or funded by the IRSST, subscribe to Prévention au travail, the free magazine published jointly by the IRSST and the CSST. Subscription: Legal Deposit Bibliothèque et Archives nationales 2010 ISBN: (print format) ISBN: (PDF) ISSN: IRSST Communications Division 505, De Maisonneuve Blvd West Montréal (Québec) H3A 3C2 Phone: Fax: Institut de recherche Robert-Sauvé en santé et en sécurité du travail, July 2010
3 Chemical Substances and Biological Agents Studies and Research Projects REPORT R-656 Engineered Nanoparticles Current Knowledge about OHS Risks and Second Edition Disclaimer The IRSST makes no guarantee regarding the accuracy, reliability or completeness of the information contained in this document. In no case shall the IRSST be held responsible for any physical or psychological injury or material damage resulting from the use of this information. Note that the content of the documents is protected by Canadian intellectual property legislation. This publication is available free of charge on the Web site. Claude Ostiguy and Brigitte Roberge, Research and Expertise Support Department, IRSST Catherine Woods and Brigitte Soucy, IRSST/University of Montréal Note : The following people have participated to the First Edition of this report published in 2006 by the IRSST in the Research and Studies Series, report # R-455. Some of the informations of this report have been kept, removed, modified, updated, or summarized in the current report. Claude Ostiguy, project leader, Research and Expertise Support Department, IRSST Gilles Lapointe, Répertoire Toxicologique, CSST Luc Ménard, Prevention-Inspection Department, CSST Yves Cloutier, Strategic Watch and Quality Management Department, IRSST Mylène Trottier, Consultant, Proximeduc Michel Boutin, Research and Expertise Support Department, IRSST Monty Antoun, Documentation Center, CSST Christian Normand, Consultant for NanoQuébec This study was financed by the IRSST. The conclusions and recommendations are those of the authors.
4 IN CONFORMITY WITH THE IRSST S POLICIES The results of the research work published in this document have been peer-reviewed.
5 IRSST - Engineered Nanoparticles: Current Knowledge about Occupational Health and Safety Risks and i SUMMARY Nanotechnology is a dynamic field and new products containing nanoparticles are being marketed every week. Already, more than 1000 are commercially available. This being the case, the development of these nanoparticles, their industrial preparation and their integration into different products involve a potential occupational exposure of hundreds of Québec workers. New Québec companies are introducing this field, thus increasing the number of potentially exposed workers. This trend should continue for several years. An initial assessment of the state of scientific knowledge about the occupational health and safety aspects (OHS) related to synthetic nanoparticles (NP) was published by the IRSST in 2006 and covered the scientific literature until the end of What was found was that OHS knowledge was very fragmentary but that research in this field was rapidly growing. This current document aims to assess the state of current knowledge in this field and summarizes the data available until early Overall, what emerges is that NP remain an important source of concern in OHS. In fact, not only does the diversity of commercially available chemical products of nanometric dimensions continue to increase, but also, the information available about the hazards specific to these substances is still very fragmentary. The literature gives us very little information specific to NP relating to their physical hazards like fires or explosions. As for health hazards, many toxicological studies on different substances have demonstrated toxic effects on various organs. It is found that in general, an NP will normally be more toxic than the same chemical substance of larger dimensions, but it is currently impossible to determine which measuring parameter for exposure is best correlated with the measured effects. The evaluation of occupational exposure must therefore address a series of different parameters, and the exposure data available are relatively rare. It should also be noted that at the present time, attention is particularly focused on carbon nanotubes (CNT), which seem to show, in different animal studies, toxicity similar to that of asbestos and consequently causing great concern in the international scientific community, mainly relating to prevention. In a context of incomplete data for the majority of nanometric substances, it remains impossible to quantify the risks for workers in the majority of situations because the toxicity of the products, the level of dust contamination of workplaces, or their potential to cause fires or explosions remain not extensively documented or totally undocumented. Nevertheless, the majority of the means of exposure control for ultrafine particles should be effective against NP and much research is currently being carried out to confirm this. In a context of uncertainty about the risks, and with an increasing number of potentially exposed workers, the current report paints a big picture of the OHS knowledge currently available in the NP field. In the absence of specific standards, a preventive and even a precautionary approach are recommended, and a review of the available means for minimizing worker exposure is presented. The needs for developing new knowledge are enormous and the authors propose some avenues of research that they feel are a priority in the current Québec context.
7 IRSST - Engineered Nanoparticles: Current Knowledge about Occupational Health and Safety Risks and iii TABLE OF CONTENTS SUMMARY... i TABLE OF CONTENTS... iii LIST OF TABLES... vi LIST OF FIGURES... vi 1. CONTEXT AND OHS ISSUES OBJECTIVES METHODOLOGY TERMINOLOGY, CLASSIFICATION, PROPERTIES AND CHARACTERISTICS OF NANOPARTICLES Terminology Classification and Properties The Main Carbon-Based Nanoparticles Fullerenes Graphene Nanofoils Carbon Nanotubes Carbon Nanofibres Carbon Black Carbon Nanofoams Other Inorganic Nanoparticles Metals Metal Oxides Quantum Dots Organic Nanoparticles Organic Polymers Biologically-Inspired Nanoparticles DEVELOPMENT, PRODUCTION AND USE OF NANOPARTICLES Efforts in Research and Development Manufacturing Processes Applications of Nanotechnologies by Sectors of Activity Nanotechnology Applications by Nanoparticle Type HEALTH AND SAFETY RISKS Health Risks Related to Specific Nanoparticles Scopes and Limits of the Current Toxicity Data Related to Nanoparticles Pulmonary Deposition of Ultrafine Dust Particles Elimination of Dusts Deposited in the Lungs Effects of Inhaled Fine Dusts and Ultrafine Dusts Epidemiological Studies Discussion on the Health Risks Safety Risks Linked to Nanoparticles...34
8 iv Engineered Nanoparticles: Current Knowledge about Occupational Health and Safety Risks and - IRSST 7. NANOMATERIALS AND THEIR AIRBORNE BEHAVIOUR AND DETECTION Definition Formation and Behaviour of Nanometric or Ultrafine Particles Detection of Nanoparticles NANOPARTICLE EXPOSURE ASSESSMENT Risk of Occupational Exposure during Nanoparticle Synthesis by Conventional Processes Measurement of Occupational Exposure during Synthesis of Nanoparticles by Conventional Processes Occupational Exposure during use of Nanoparticles EXPOSURE PREVENTION AND CONTROL Prevention Toxic Risk Assessment The Control Banding Approach Risk Control and Nanoparticle Control Strategies Personal Protection Prevention of Fires, Explosions and other Risks Risks of Catalytic Reactions, Explosion and Fire Key Factors Risk Characterization Risk Reduction / Explosion Prevention Risk Reduction / Fire Prevention Catalytic Reactions Storage Routine Maintenance and Workplaces Spills Waste Disposal Other Aspects of Prevention REGULATION AND RECOMMENDATIONS Necessary Ethical Rules Regulation in European Nations and the European Community Asia-Pacific Region North America The United States Canada Québec THE MAIN ACTORS IN QUEBEC...97
9 IRSST - Engineered Nanoparticles: Current Knowledge about Occupational Health and Safety Risks and v 12. POTENTIAL AVENUES OF RESEARCH The Main Orientations for Developing Research in the World The Main Research Development Avenues proposed to the IRSST DISCUSSION CONCLUSION BIBLIOGRAPHY...119
10 vi Engineered Nanoparticles: Current Knowledge about Occupational Health and Safety Risks and - IRSST LIST OF TABLES Table 1: Examples of Properties sought through the Use of Nanoparticles in Different Economic Activity Sectors...17 Table 2 : Some Examples of Nanoparticle Applications...18 Table 3 : Main Parameters Allowing the Proper Characterization of Nanoparticles for Toxicological Studies...24 Table 4 : Elimination of Dusts Deposited in the Lungs (Synthetic Table)...28 Table 5 : Nanoparticle Coagulation Time as a Function of their Size and Concentration...42 Table 6 : Examples of Instruments and Techniques Allowing Characterization of NP Aerosols...52 Table 7 : Types of Electron Microscopes which Can Contribute to NP Characterization...54 Table 8 : Risks of Exposure to Nanoparticles during their Synthesis...56 Table 9 : Comparison of Assigned Protection Factors of Respirators (USACHPPM )...73 LIST OF FIGURES Figure 1 : Schematic Representation of a Fullerene C Figure 2 : Schematic and Visual Representation of a Quantum Dot...9 Figure 3 : Percentage Distribution of the Expected Global Economic Impact of Nanotechnologies in Figure 4 : Standard Curves for Airway Dust Penetrating the Pulmonary Airways...26 Figure 5 : Prediction of Total and Regional Deposition of Particles in the Airway, by Particle Size...27 Figure 6 : Potential Effects of Inhaled Ultrafine Particles...33 Figure 7: Explosion Hexagon...37 Figure 8: Examples of Conditions Favouring the Occurrence of an Explosion...37 Figure 9 : Distribution of the Diameters of Particles Commonly Found in Workplace Air...40 Figure 10 : Relationship between the Numerical Concentration of Particles and the Time Required to Coagulate...41 Figure 11 : Variables and Physico-Chemical Characteristics of Nanoparticles Useful for Risk Assessment...43 Figure 12 : Some Techniques Usable for Airborne Dust Characterization...44 Figure 13 : Classic Approach to Risk Assessment...66 Figure 14 : Risk Control Hierarchy Applied to NP...70 Figure 15 : Parameters Contributing to the Efficiency of Air Purification Elements...74
11 IRSST - Engineered Nanoparticles: Current Knowledge about Occupational Health and Safety Risks and 1 1. CONTEXT AND OHS ISSUES The field of nanotechnology (NT) is changing rapidly, and in the near future should have a profound effect on every sector of society. This is why a number of authors maintain that it constitutes a third industrial revolution, following the mechanization and computerization revolutions. As such, the industrialized countries -- quite rightly -- see the nano-world as showing great promise in economic development and spinoffs. Governments, as well as large firms, are developing strategic plans and investing considerable sums in research and development (R & D). Europe, for example, has made nanotechnology one of its seven priority areas in its targeted research, and has invested 1.3 billion Euros in it for the period (www.cordis.lu/nmp/home.html) 1. For the year 2008 alone, the National Nanotechnology Initiative (NNI) in the United States had a budget of 1.49 billion dollars (NNI, 2008). Canada, too, has invested in the design, manufacture and uses of NT (Chapter 5). Yet what exactly are NT? The prefix nano signifies a billionth (10-9 ). Thus, a nanometre (nm) is a billionth of a metre. Nanotechnology is concerned with the creation or handling of particles and materials that, as a minimum: (i) have one nanometric dimension, normally 1 nm to 100 nm, and (ii) are produced through the structured organization of groups of atoms and molecules, or through reduction, at the nanometric level, of macroscopic materials. The interest in NT is essentially based on the fact that certain particles reveal specific properties only when they are of nanometric dimensions. These properties may include chemical, biological, electronic, rheological, magnetic, optical (photon), mechanical and structural effects. Although the development of NT is a modern multidisciplinary science, naturally produced and manmade materials of nanometric dimensions and exposure to particles of other dimensions of mineral or environmental origin, including the fine fraction of nanometric particles, have always existed. Some of the natural nanometric particles are of biological origin including DNA with a diameter of around 2.5 nm and many viruses (10 to 60 nm) and bacteria (30 nm to 10 μm) while others are found in desert sand, oil fumes, smog, and fumes originating from volcanic activity or forest fires and certain atmospheric dusts. Among those generated by human activity, we should mention diesel fumes, industrial blast furnace emissions and welding fumes, which contain particles of nanometric dimensions (Teague, 2004). However, basing the definition of NP on their size may induce too broad an understanding of our field of research. It is therefore essential to set limits for the object of our study. In this report, the term nanoparticles (NP) will be used to describe particles from 1 to 100 nm, synthesized intentionally with an objective of commercial use of one of the unique properties at these dimensions. Note that an ISO standard, which was at the ballot stage at the time of the final writing of this document, proposes a different terminology. It is suggested that the term nanomaterials be used, which includes nano-objects as well nanostructured materials, with the latter being nonnanometric objects but having a fine nanometric-dimension structure. Nano-objects consist of a) nanoparticles whose three dimensions are nanometric, b) nanofibres (nanowires, nanotubes and nanorods) having two nanometric dimensions, and c) nanoplates with only one nanometric 1 At the time the report was in preparation, all the websites cited were in operation.
12 2 Engineered Nanoparticles: Current Knowledge about Occupational Health and Safety Risks and - IRSST dimension. Despite this situation, the editorial committee for this document decided to retain the nanoparticle terminology in order to maintain continuity with the studies published earlier by the IRSST and so as not to confuse the readers of this document with new terminology, not yet in common use in the scientific literature. Therefore, the term nanoparticle (NP) used in this document refers only to synthetic NP and consists of all of the elements in the nano-object group proposed in this new ISO standard. In the past few years, we have noted an awareness of the urgency of developing knowledge relating to synthetic NP risks for occupational health and safety (OHS) and for the environment and public health in general. To all indications, we currently have limited knowledge of OHS specific to NP, primarily due to a lack of information on toxic risks occupational exposure and working conditions. Even if it is also possible to measure exposure with the technologies currently available, our ability to predict the impact on workers health is therefore very limited. However, various NP are already coming onto the market after manufacturing. There are already more than 1000 commercialized products containing nano components. The manipulation of these materials in the work environments generates some concerns and raises questions regarding the risks to workers health and safety. The purpose of this document is to report on our current knowledge. The present document is intended primarily to serve as a source of information for anyone seeking to understand NP, what they are used for and, above all, the occupational health and safety issues related to their synthesis and handling. Thus, the information summarized here could be of interest to a wide variety of groups, including not only occupational health and safety professionals, but also researchers, evaluation- and risk-management specialists, employers and decision makers in industry, governmental agencies that develop policies, laws and regulations, as well as workers who may be potentially exposed and the general population wishing to find out more on the subject. In order to limit the length of this document, some information already presented in the first edition will be summarized here, and the reader interested in more detailed information can consult the IRSST report (http://www.irsst.qc.ca/files/documents/pubirsst/r-455.pdf), (Ostiguy et al., 2006b).
13 IRSST - Engineered Nanoparticles: Current Knowledge about Occupational Health and Safety Risks and 3 2. OBJECTIVES The principal objective of the study is to draw an overall portrait of knowledge on NP, emphasizing OHS and prevention aspects. In no way should this document be considered a critical analysis of the existing scientific literature. Amongst other things, we will describe (i) the principal known health risks and impacts, (ii) safety risks, (iii) the characteristics, exposure assessment and control of these risks, as well as OHS research needs relevant to the field of NT. The report also seeks to strengthen Québec expertise in the field. This expertise should provide effective support to research teams and institutions synthesizing or using these products. 3. METHODOLOGY The initial literature review of available information up to the end of 2004 had allowed us to observe the rapid changes in knowledge occurring in the field of OHS dealing with NP. In light of the fact that the methodology employed at that time enabled us to reach our objective, it has been retained to produce the second edition, which covers the scientific literature up to early Consequently, the present report is based on: analysis of the scientific literature that uses approaches commonly used for this type of research; these approaches are found in journals with peer committees. The IRSST Information Library and the CSST Information Resource Centre conducted the literature search. The principal data banks and search engines consulted were MedLine, Toxline, PubMed, Inspec, Coppernic, Embase, Ntis, Ei, Compendex, SciSearch, Pascal, Alerts, Teoma and Scirus. A number of keywords (in both French and English) were used, including nanotoxicology, nanotechnology, nanoparticle, nanomaterial, health effects, explosion, fire, toxicity and toxic. This information was particularly useful in documenting the toxicity of nanoparticles; an Internet search, primarily to document (i) the types of processes facilitating the manufacture of these products, and (ii) the description of these products, their properties and their potential uses; the use of scientific reviews by recognized committees of international experts in the fields of nanoparticles and nanotechnology; information collected from Quebeckers directly involved in the nanotechnology field; discussions with the editorial committee of the report.
15 IRSST - Engineered Nanoparticles: Current Knowledge about Occupational Health and Safety Risks and 5 4. TERMINOLOGY, CLASSIFICATION, PROPERTIES AND CHARACTERISTICS OF NANOPARTICLES 4.1 Terminology As discussed previously, NP are products that have been synthesized because they have unique properties relating specifically to their dimensions. Moreover, in recent years substantial progress has been made in defining them, especially through the creation of groups of experts working in the area of standards development. Today, an international consensus exists. Recent studies by British Standards Institute (BSI, 2005), the American Society for Testing and Materials (ASTM, 2006), the Nordic group (Schneider et al., 2007) and the ISO (2008a) have defined NP as particles with one or several dimensions of 1 to 100 nm. By contrast, terminology surrounding various aspects of NT continues to be the subject of debate as described in chapter 1. One-dimensional systems, such as thin films or manufactured surfaces, have been used for decades in the electronics, chemical and engineering industries. Production of thin or monolayer films is now common practice in the electronics field, as is the use of made-to-measure surfaces for solar cells or catalysis. These fields are known and the risks are normally well controlled. The properties of two-dimensional systems (carbon nanotubes (CNT), inorganic nanotubes, nanowires, nanofibrils and biopolymers) are less well understood and the manufacturing capabilities are less advanced. Finally, some 3D systems are well known, such as metal oxides, carbon black, titanium dioxide (TiO 2 ) or zinc oxide (ZnO), particles, precipitates, colloids and catalysts of nanometric dimensions, while others, such as fullerenes, dendrimers and quantum dots, currently pose major challenges in terms of production and understanding of their properties. The question of NP dimensioning is crucial, because the properties of nanostructures are directly related to those of individual molecules instead of those of bulk materials (Kohler and Fritzche, 2004; Royal Society and Royal Academy of Engineering, 2004). In fact, NP are observed to have radically different, even unique properties at nanometric dimensions: exceptional strength, programmable electrical conductivity, unsuspected optical properties, etc. The very principles of chemistry and classical physics of solid materials must be replaced by quantum approaches based on the probabilities that each atom, each molecule, can play a determining role and that the interactions among them have a decisive impact on the behaviour of the whole. Thus, the classical mechanical parameters of solids no longer prevail. In fact, it is the individual molecular and atomic dimensions and interactions that determine the arrangement, stability, flexibility and function of nanostructures. Two central factors seem to be responsible for the changes in properties observed in NP: a much larger relative surface per unit of mass and a predominance of quantum effects. The first factor is responsible for the changes in reactivity, which may increase considerably with a decrease in the size of NP. The second factor, observed for certain particles of a few nm or tens of nm, induces changes in optical (photonic), electrical, electronic, mechanical, chemical, biological, rheological, structural or magnetic properties.
16 6 Engineered Nanoparticles: Current Knowledge about Occupational Health and Safety Risks and - IRSST Once the dimensions are determined, a simple way to classify NP is to group them by chemical composition, and this is the approach we will use. However, we should mention that many NP are coated immediately after synthesis to prevent any aggregation and preserve their properties. These modifications, in return, may have a direct impact on their composition, size and reactivity. 4.2 Classification and Properties In view of the objective of our report and the fact that production of new nanomaterials is a fastgrowing field of research, only the most common products will be described briefly. For more details, it is recommended that you consult the special edition of the Journal of Materials Chemistry regarding preparation of nanomaterials (Rao, 2004). Rao et al. (2004) have also published a volume describing the theory, synthesis, properties and applications of these products. Many specialized journals have also emerged in the last decade and new NP structures with novel properties are reported regularly in these publications. The reader can also consult the first edition of the IRSST report (http://www.irsst.qc.ca/files/documents/pubirsst/r-455.pdf; Ostiguy et al., 2006b) The Main Carbon-Based Nanoparticles Fullerenes Fullerenes are spherical cages composed of carbon atoms, which are bound to three other atoms in sp 2 hybridization (Figure 1). The most widely studied form, synthesized for the first time in 1985 (Kroto et al.), is spherical and contains 60 carbon atoms, C 60, although there have been reports of structures containing 28 to 1500 carbon atoms, which can reach a diameter of 8.2 nm. Formation of multilayer fullerenes has also been reported, with dimensions potentially ranging from 4 to 36 nm (Sano et al., 2002). Figure 1 : Schematic Representation of a Fullerene C 60
17 IRSST - Engineered Nanoparticles: Current Knowledge about Occupational Health and Safety Risks and 7 Given their interesting properties, it has been suggested that they be used in the electronic field, in batteries, solar cells and combustion cells, for data storage or gas storage, or as additives in plastics. Incorporating them into carbon nanotubes (CNT) modifies the electrical behaviour of fullerenes, creating regions with varying semiconductive properties, thus offering potential applications in nanoelectronics. Their optical properties vary according to wavelength, thus finding applications in telecommunications. Since fullerenes are empty structures with dimensions similar to several biologically active molecules, they can be filled with different substances and find medical applications, particularly in the therapeutic field against cancer or AIDS Graphene Nanofoils Graphite is composed of a series of superimposed layers of a hexagonal network of carbon atoms, in which each atom is bound by three neighbouring carbon atoms in a planar network. Separating these layers into a monolayer around one nanometre thick makes it possible to obtain graphene foils. This allows unique electronic, magnetic, optical and mechanical properties to appear. Applications are currently envisioned in recovery and in the flexible electronic components field Carbon Nanotubes Carbon nanotubes (CNT) are a new crystalline form of carbon. Wound in a hexagonal network of carbon atoms constituting a graphene nanofoil, these hollow cylinders can have diameters as small as 0.7 nm with lengths that can range from a few micrometres, and reach several millimeters in length (Hett, 2004a). Each end can be opened or closed by a fullerene halfmolecule. These nanotubes can have a single layer (SWCNT for single walled carbon nanotube) or several layers (MWCNT for multi walled carbon nanotube) of coaxial cylinders of increasing diameters in a common axis. Multilayer carbon nanotubes can reach diameters of 100 nm (Aitken et al., 2004). Endo (1986) seems to have been the first to report the existence of CNT. They display metallic or semiconductive properties, depending on how the carbon leaf is wound on itself. The substitution of carbon atoms allows modification and adjustment of electronic properties. The current density that a nanotube can carry is extremely high and can reach one billion amperes per square metre (Pautrat, 2003, Aitken et al., 2004). Light and flexible, chemically very stable and totally insoluble, mechanical resistance under tension, CNT is more than sixty times greater than that of the best steels, even though they weigh six times less (Aitken et al., 2004). They also present a very large specific surface area, and a great capacity for molecular absorption (Maynard, 2004). The different processes of synthesis, purification and post-synthesis treatment will lead to products displaying very different properties (Helland et al., 2007). CNT are ranked among the most promising materials and researchers have detected a whole range of potential CNT applications in nanotechnology: polymer composites, electron transmitters, electromagnetic armouring, supercapacitors, storage of gases, including hydrogen, batteries, structural composites (Eklund et al., 2007) Carbon Nanofibres Just like CNT, carbon nanofibres are composed of graphene foils. But unlike nanotubes, they do not wind into a regular cylinder. Instead they form a cone-shaped or cup-shaped structure. In
18 8 Engineered Nanoparticles: Current Knowledge about Occupational Health and Safety Risks and - IRSST view of these particularities, the mechanical and electrical properties of nanofibres will be different than those of CNT. Their use is envisioned as additives in polymers, as catalytic media and for gas storage Carbon Black Carbon black is composed of partially amorphous graphitic material, with a substantial fraction of the elementary particles of nanometric dimensions, generally from 20 to 70 nm. These particles, mostly spherical, are bound in aggregates that interact strongly with each other to form agglomerates of up to 500 nm. These are often marketed in the form of pastilles or blocks and have been used in very high volumes for the past few decades, mainly as pigments and strengthening agents in rubber, particularly for tires. This technology is well known, and it is only partly covered in the report Carbon Nanofoams Carbon nanofoams are the fifth known allotrope of carbon, after graphite, diamond, carbon nanofibers and fullerenes. In carbon nanofoam, islands of carbon atoms, typically from 6 to 9 nm, are randomly interconnected to form a very light, solid and spongy three-dimensional structure, which can act as a semiconductor. Carbon nanofoams display temporary magnetic properties (Health and Safety Executive, 2004b) Other Inorganic Nanoparticles Metals Most metals have been or can be produced in nanometric dimensions. Among them, gold NP are studied in particular and show an optical resonance spectrum in the visible range, which is sensitive to the environmental conditions, size and shape of NP. Their unique properties make it possible to envision a series of applications, particularly as optical markers for medical diagnosis or as cancer treatment agents. Nanometric silver is also produced in large quantities and is mainly used for its antimicrobial properties (ICON 2008; Hansen 2009). Nanometric platinum, palladium and rhodium are used in catalytic converters, iron, nickel and cobalt as catalysts, particularly for the synthesis of carbon nanomaterials, aluminium as a fuel, iron as a doping metal and copper in electronics. Gold, copper, silicon and cobalt nanowires, capable of being electrical conductors or semiconductors, have also been perfected and could be used to transport electrons in nanoelectronics. Finally, nanowires have been developed based on different metals, oxides, sulphides and nitrides Metal Oxides Several metal oxides of nanometric dimensions have been created, but the most common ones, because they are produced on a large scale, are probably silica, titanium dioxide and zinc oxide. They are used either natural or coated, mainly in the fields of rheology, plastics and rubbers as active agents and additives (SiO 2 ), in sun creams (TiO 2, ZnO), and as pigment in paint (TiO 2 ). Different metal oxides have appeared in varied forms: nanotubes, nanorods, nanoflakes, etc. In addition, certain structures show interesting properties for virtual applications in fields such as
19 IRSST - Engineered Nanoparticles: Current Knowledge about Occupational Health and Safety Risks and 9 sensors, optoelectroics, transducers and medicine Other metal oxides are also produced, including cerium, iron, copper, zirconium, aluminium, nickel, antimony, yttrium, barium and manganese oxides, as well as nanoclays (ICON 2008) Quantum Dots An important field of research, for the past fifteen years, quantum dots are typically composed of combinations of Group II and IV elements or Group III and V elements of the periodic table. They have been developed in the form of semiconductors, insulators, metals, magnetic materials or metallic oxides. The number of atoms in quantum dots, which can range from 1,000 to 100,000, makes them neither an extended solid structure nor a molecular entity (Aitken et al., 2004). With smaller dimensions than the exciton Bohr radius, they display unique optical and electronic properties at diameters of about one to ten nm. Because of their quantum confinement, they can, for example, absorb white or ultraviolet light and reemit it at a specific wavelength a few nanoseconds later (Aitken et al., 2004). Depending on the composition and size of the quantum dot, the light emitted may range from blue to the near infrared. The flexibility of quantum dots and their associated optical properties make it possible to envision applications in fields such as multicolour coding in the study of genetic expression, in high-resolution and high-speed screens and in medical imaging. Their high surface-to-volume ratio allows them to be combined with antibodies, proteins and oligonucleides (Michalet et al., 2005). Some quantum dots are modified to produce drug vectors, diagnostic tools and inorganic solar batteries (Akerman et al., 2002; Michalet et al., 2005). Figure 2 : Schematic and Visual Representation of a Quantum Dot Organic Nanoparticles Organic Polymers Many common organic polymers can be produced in nanometric dimensions. The polyvinyl chloride or latex thus produced, for example, can be solubilized or modified chemically under certain conditions. Some of these organic polymers can be prepared in the form of nanowires, resulting in their use in the development of liquid-phase or gas-phase ultrafiltration systems, or particularly as sensors. Some biodegradable organic nanofibres could be used in medicine for tissue reengineering or bone regeneration or to control the release of drugs. New structures have also been synthesized, such as dendrimers, which represent a new class of controlled-structure polymers of nanometric dimensions. These dendrimers are synthetic threedimensional macromolecules developed from a monomer, deploying and multiplying new
20 10 Engineered Nanoparticles: Current Knowledge about Occupational Health and Safety Risks and - IRSST branches in successive tiers, until a synthesized symmetrical structure is constituted (ICON, 2008). They are considered to be basic elements for the large-scale synthesis of organic and inorganic nanostructures of dimensions ranging from 1 to 100 nm and exhibit unique properties. Dendrimers allow precise, atom by atom control of nanostructure synthesis, based on the dimensions, shape and desired surface chemistry. Given that they can be designed as hydrophilic or hydrophobic, their use can be highly diversified. With different reactive surface groupings, it is envisioned that dendrimers will be used extensively in the medical and biomedical field as a means of delivering drugs and nutraceutics, as therapies, for biotests or as imaging contrast agents (Tomalia, 2004; ICON, 2008). Compatible with organic structures such as DNA, they can also be manufactured to interact with metal nanocrystals and nanotubes or be encapsulable or show unimolecular functionality (Tomalia, 2004). Their use is also anticipated as an ink in printers, as a metallic chelating agent in ion exchanger resins, in coatings, in cosmetics or as a viscosity modifier or environmental rehabilitation substance (ICON, 2008) Biologically-Inspired Nanoparticles Biologically inspired NP are highly diversified but normally include structures in which a biological substance is encapsulated, trapped or absorbed on the surface. In particular, lipids, peptides and polysaccharides are observed, used as vector for the targeted transport of drugs, receptors, medical imaging chemicals or nucleic acids. For example, liposomes, micelles or polyplexes are found, some of which may come from natural materials, while others are synthesized. These structures, widely studied in the medical and pharmacological field, will not be discussed in this document, given the lack of information available regarding them in the scientific literature dealing with OHS.